Kodai Kuwata · Yukie Saito · Satoshi Shida Masamitsu Ohta
Intercalation of wood charcoal with sulfuric acid
Abstract Intercalation of wood charcoal with sulfuric acid (H2SO4) was investigated. Carbonized sugi (Japanese cedar) samples were prepared by heating at various temperatures in the range 1700°–2700°C. Electrochemical oxidization was carried out in H2SO4 and the feasibility of intercalation was determined. In potentiometric analysis, plateaus appeared for samples carbonized at temperatures above 2300°C. In their X-ray diffraction profi les, the peak at around 26° was shifted to a smaller angle of about 22.4°. These results can be considered as signs of intercalation with acid molecules. Fourier transform infrared analysis of charcoal heated at 2700°C, following washing with water and drying of the sample, showed a band at 1220 cm−1
that was assigned to a sulfonate group. This band was not observed for samples heated at 1900°C. These observations suggest the occur-rence of intercalation in the former charcoal, but not in the latter. It is concluded that wood charcoal can undergo inter-calation when it has ordered stacking of hexagonal carbon layers.
Key words Wood charcoal · Intercalation · X-ray diffrac-tion · Thermogravimetry · FT-IR
Wood charcoal is a potential source of carbon material. The main product of wood charcoalization is carbonized cell walls, which is nongraphitic carbon. Generally, nongraphitic
K. Kuwata · Y. Saito (*) · S. Shida · M. Ohta
Graduate School of Agricultural and Life Sciences, The University of Tokyo, 1-1-1 Yayoi, Bunkyo-ku, Tokyo 113-8657, Japan
Tel. +81-3-5841-5246; Fax +81-3-5684-0299 e-mail: email@example.com
Part of this article was presented at the 55th, 56th, and 57th Annual Meetings of the Japan Wood Research Society, Akita, Hiroshima, and Tsukuba, August 2006, August 2007, and March 2008, respectively, and at the International Conference on Carbon “CARBON 2008,” Nagano, July 2008
carbon cannot develop into perfect graphite crystals even if it is annealed at temperatures as high as 3000°C, because of restriction by the growth history of solid-phase carboniza-tion. However, carbonized wood cell walls are expected to be a carbon source for future applications, having various allotropic structures, such as onion-like structures1 and dia-monds.2
By using approaches considering the characteristic features of wood charcoal, novel functional materials should be obtainable. There is a concept of reducing CO2 emissions in air by returning pyrolyzed biomass to the soil as biochar.3,4 In future, this concept could be extended to sequestration of carbon not only in soil, but also in industrial carbon materials. For this extended “carbon offset,” trials making carbon materials from biomass illustrate an important approach. As one such approach, we have made intercala-tion compounds of wood charcoal.
A well-known graphite intercalation compound is a lamellar crystal-like structure, with guest molecules inserted between the ordered stacking of hexagonal carbon layers. Predominantly, the graphite–H2SO4 intercalation com-pound is the source for “exfoliated graphite,” with a low bulk density. It is used in industrial materials such as coating agents, additives, and fl exible graphite. At present, exfoli-ated graphite is considered to have potential use as an oil absorbent and in heat-resisting applications.
To date, intercalation of “nongraphitizing carbon,” including wood charcoal has scarcely been reported, while much research on graphitic carbon from petroleum sources has been carried out and applied. This is probably because synthesis of intercalation compounds requires perfect crys-tallinity and a large crystallite size of graphite;5
in short, the driving force is the charge-transfer interaction that occurs in orderly stacked hexagonal carbon layers in highly crystal-line graphite. However, by treatment at relatively high tem-peratures like 2000°C or higher, even nongraphitic carbon such as wood charcoal includes a mosaic graphitic portion or turbostratic portion. These portions have orderly stacked hexagonal carbon layers, but do not contain perfectly crys-talline graphite. We considered that these highly ordered portions in wood may be suitable to form intercalation compounds. The aim of this study was to clarify whether
wood charcoal can form intercalation compounds when it contains some degree of graphitic structure.
Materials and methods
Sugi (Japanese cedar, Cryptomeria japonica) was precar-bonized using a traditional stone kiln at a temperature of 1200°C. Samples were cut into blocks of several cubic cen-timeters and placed in a small carbon crucible. The crucible was placed in a furnace (SCC-30/220, Kuratagiken, Japan), where the thick-walled carbon crucible served as the electri-cal resistance heater element. For secondary carbonization, samples were heated at a rate of 60°C/min, held for 1 h at 1700°, 1900°, 2100°, 2300°, 2500°, or 2700°C and then cooled at a rate of 120°C/min. During the thermal treatment, the ambient pressure was kept at 10–20 Pa by evacuating the furnace, but at temperatures above 1900°C a fl ow of argon gas was introduced and maintained at a pressure of 0.105– 0.11 MPa. After treatment, the sample was powdered and sieved to give a powder with a particle diameter of less than 63 μm. Natural graphite (Wako, Japan) was also used in subsequent tests.
Electrochemical treatment and potentiometry
The powdered sample was stuffed into a cell in contact with a Pt electrode and was placed as the anode immersed in H2SO4. During treatment, the test tube was kept at 30°C in a thermostatic chamber and dried N2 gas was purged inside to prevent absorption of moisture by H2SO4. Electrochemi-cal treatment and potentiometry were achieved under a constant electric current of 200 μA. After 20 h for stabiliza-tion, potentiometry was started and continued until the potential reached equilibrium. The maximum increment of the potential was 2.3 to 2.5 V.
Diffractometry was achieved by using a RINT2000 diffrac-tometer (Rigaku, Japan) with a 40 mA/40 kV CuKa beam, taking 41 min to move between 15° and 35° at intervals of 0.04°. The resultant diffractogram was quite noisy due to the short measurement time, which was necessary to mini-mize oxidation and moisture absorption of the samples wetted with H2SO4 on exposure to air. Noise in the diffrac-tograms was reduced by Savitsky-Golay smoothing. Accord-ing to a previous report,6
the peaks were divided by a Gaussian-Lorenzian approximation and the thickness of carbon layer stacks (Lc) was calculated from the half width by using Sherrer’s equation.
After electrochemical treatment, the samples wetted with H2SO4 were immediately placed in a Pt pan and differential
thermal analysis (DTA) and thermogravimetric analysis (TGA) were performed simultaneously with a Thermo Plus (Rigaku) at a heating rate of 5°C/min under a fl ow of dried N2. For comparison, samples not subjected to electrochemi-cal treatment were also immersed in H2SO4 prior to DTA/ TG measurements.
Fourier transform infrared spectroscopy
The electrochemically treated samples were washed with water and dried. For each sample, a small amount of less than 1 mg was dispersed in a matrix of KBr (200 mg) and pressed to form a pellet. Fourier transform infrared (FT-IR) spectra were recorded as KBr disks on a Nicolet Magna 860 FTIR spectrometer under a fl ux of dried air.
Electrochemical treatment and potentiometry
The progress of the reaction was traced by in situ measure-ment of electrical potential, following the method of Iwashita and Inagaki.7 Using potentiometry, intercalation should be recognized as stepwise increase of electric poten-tial. Under such electrical treatment, graphite undergoes several stages of intercalation compounds, with different energy levels. The appearance of plateaus in the potential curve means that intercalation has advanced to the next stage. When intercalation reaches the fi nal stage, the elec-tric potential stops increasing. As shown for natural graph-ite in Fig. 1, plateaus can be observed in the potential curve in the course of reaching equilibrium. The plateaus were clearly observed for sugi samples carbonized at 2300°C or higher temperatures (arrowed regions in Fig. 1, 2300°, 2500°, and 2700°C). However, for samples carbon-ized at temperatures less than 2100°C, no clear plateau could be observed. The appearance of a plateau implies that for the sugi samples carbonized at 2300°C and higher temperatures, intercalation compounds with H2SO4 can be formed.
X-ray diffractograms of the samples before electrochemical treatment show that turbostratic and graphitic structure appeared at carbonization temperatures higher than 2300°C (Fig. 2A) as mentioned in a previous report.6
Wood char-coals treated at 2300°C or higher temperatures probably have orderly stacked carbon layers that can form inter-calation compounds. Iwashita and Inagaki7
In Fig. 2B, the (002) refl ection for natural graphite just after electrochemical treatment, marked as G in Fig. 2A, disappeared and a new peak appeared at 2q= 22.4°, corre-sponding to 0.397 nm. This is a diagnostic peak for inter-calation of H2SO4 with a molecular size of about 0.460 nm. When H2SO4 is inserted between the stacked carbon layers with an original separation distance of 0.335 nm, the tance increased to 0.795 nm, which is twice the original dis-tance. For the sugi samples, although the refl ection by a large amorphous region overlaps and makes the refl ection of the ordered portion unclear, a new peak around 22.4° is
clearly observed for samples treated at 2300°C or higher. This indicates the occurrence of intercalation.
Figure 3 shows DTG and DTA curves, in which all samples for traces b–g had peaks at 200° to 250°C. These are con-sidered to be due to evaporation of H2SO4, because a similar peak appeared for genuine H2SO4 (trace a in Fig. 3). The shape of the peaks is very similar for DTG and DTA, but different among samples, possibly because the endothermic energy for the evaporation reaction of H2SO4 depends on the samples. It is possible that interactions between H2SO4 and the sample surface vary according to the carbonization temperature. The other possibility is that during the proce-dure, H2SO4 may introduce water from the air in varying amounts. On the other hand, another peak was observed at around 130°C in the exothermic reaction, but only for the sugi sample carbonized at 2700°C and for graphite after electrochemical treatment (traces f and g in Fig. 3). This peak is possibly due to intercalated H2SO4. The peak around this temperature is known, at which point the graphite intercalation compound changes into exfoliated graphite, where the trapped H2SO4 between the stacked carbon layers causes expansion and delamination of the stacked carbon layers.8
Thus, thermal analysis indicated that the sugi sample carbonized at 2700°C could form an intercala-tion compound. 2 2.5 3
)2 2.5 3
)1.5 2 2.5 3
l(V)0 0.5 1 1.5
0 10 20 30
Time(h)1.5 2 2.5 3
ntial(V)0 0.5 1 1.5
0 10 20 30
1 1.5 2 2.5 3
ential(V)0 0.5 1
0 20 40 60
Time(h)1 1.5 2 2.5 3
l(V)0 0.5 1
0 10 20 30
1 1.5 2 2.5 3
l(V)0 0.5 1
0 20 40 60
0 0.5 1
0 10 20 30
0 20 40 60 80
Fig. 1. Potentiometry curves for sugi samples carbonized at various
temperatures (1700°, 1900°, 2100°, 2300°, 2500°, and 2700°C) and natural graphite (Graphite), under electrochemical treatment in 98% H2SO4. Arrows indicate plateaus
15 20 25 30 35
In te n si ty Ic 2700 2500 2300 2100 1900 1700 In te n si ty
15 20 25 30 35
(B)c Graphite 2700 2500 2300 2100 1900 1700
15 20 25 30 35
Fig. 2A, B. X-ray diffractograms of natural graphite and carbonized
sugi samples A before and B after electrochemical treatment in 98% H2SO4. Bottom to the top: sugi samples carbonized at 1700°, 1900°,
Figure 4 shows the FT-IR spectrum of residues after elec-trochemical treatment followed by washing in water and drying. In general, the residual product from the graphite intercalating compound is known as a “residual compound,” which partially keeps sulfuric acid molecules between its carbon layers. For all samples, bands for inorganic sulfuric acid were observed at around 645, 1105, and 1155 cm−1, probably due to excess H2SO4 that did not intercalate and remained in the sample even after washing in water (Fig. 4). On the other hand, for the natural graphite and sugi samples carbonized at 2700°C, additional bands due to a
sulfonate group appeared at 1045 and 1180 cm−1
. This sul-fonate group may have been produced via a reaction between carbon on the hexagonal carbon layer and interca-lated sulfuric acid, possibly indicating intercalation of sul-furic acid between the hexagonal carbon layers (Fig. 4).
Considering the results of potentiometry, X-ray diffraction, and thermal analysis, wood charcoal treated at 2700°C appears to intercalate sulfuric acid. The results indicate that even wood charcoal, which is categorized as nongraphitiz-able carbon can form an intercalation compound when the parent wood charcoal has a well-developed stacked carbon layered structure. Wood charcoal is a product of multi-phased graphitization, including combination of sp2
- and sp3
and consists of a mixture of graphitic, turbostratic, and amorphous components. The graphitic component is considered to be the main body of the host for intercalation. By using H2SO4 as a probe to investigate the wood charcoal structure, the amorphous component was revealed to be quite sparsely packed, allowing the H2SO4 to pass through easily to reach the graphitic compo-nent. Another important point to be clarifi ed is whether the turbostratic component can also form an intercalation com-pound. In this study, the possibility was implied, but not clarifi ed. If turbostratic carbon can form intercalation struc-tures, it will have practical uses for industry because tur-bostratic carbon can be systematically produced from wood using Ni catalysts.10
Further investigations to identify which components of complicated wood charcoal can intercalate are expected to lead to future applications.
Sulfuric acid intercalation of sugi samples carbonized at various temperatures was investigated. After electrochemi-cal treatment with H2SO4, only sugi samples carbonized at 2300°C or higher temperatures showed the (002) refl ection in the X-ray diffractogram shifting to lower angles. This indicates that the stacking distance of hexagonal carbon layers was increased by intercalation. An exothermic peak at around 130°C, which is characteristic for H2SO4–graphite intercalation compounds, was observed by DTA for sugi samples that had been carbonized at 2700°C and electro-chemically treated. However, this peak was not observed for sugi samples that were carbonized at 1900°C and elec-trochemically treated, or for samples not subjected to electrochemical treatment. The results of thermal analysis indicated that intercalation occurred with sugi samples car-bonized at 2700°C. The electrochemically treated samples were washed in water and dried before FT-IR spectroscopy. For samples considered likely to show intercalation, bands due to sulfonate groups were observed and these were considered to be traces of H2SO4 intercalation. Thus, this study revealed that wood charcoal can form intercalation
100 200 300
100 200 300
Temperature(°C) ( )
Fig. 3. A Thermogravimetric and B differential thermal analysis
curves. a, H2SO4; b, sugi carbonized at 1900°C, before electrochemical
treatment; c, sugi carbonized at 2700°C, before electrochemical treat-ment; d, natural graphite before electrochemical treattreat-ment; e, sugi carbonized at 1900°C, after electrochemical treatment; f, sugi carbon-ized at 2700°C, after electrochemical treatment; g, natural graphite after electrochemical treatment. Arrows show characteristic peaks for intercalation compounds
1200 1000 800 600
Fig. 4. Fourier transform infrared spectra of residual compounds after
electrochemical treatment and washing in water and drying. a, Graph-ite; b, sugi carbonized at 2700°C; c, sugi carbonized at 1900°C. Filled
compounds when carbonized at temperatures higher than 2300°C with an ordered stack of hexagonal carbon layers.
Acknowledgments This research was partially supported by the
Ministry of Education, Science, Sports, and Culture through a Grant-in-Aid for Young Scientists (A) (Yukie Saito, 18688008, 2006–2008).
1. Hata T, Imamura Y, Kobayashi E, Yamane T, Kikuchi K (2000) Onion-like graphitic particles observed in wood charcoal. J Wood Sci 46:89–92
2. Ishimaru K, Vystavel T, Bronsveld P, Hata T, Imamura Y, Hosson JD (2001) Diamond and pore structure observed in wood charcoal. J Wood Sci 47:414–416
3. Ueno M, Kawamitsu Y, Komiya Y, Sun L (2007) Carbonisation and gasifi cation of bagasse for effective utilization of sugarcane biomass. Int Sugar J 110:22–25
4. Lehmann J (2007) Bio-energy in the black. Front Ecol Environ 5:381–387
5. Bartlett N, McQuillan BW (1982) Graphite chemistry. In: Whittingham MS, Jacobson AJ (eds) Intercalation chemistry. Academic, London, pp 19–54
6. Tanaka T, Saito Y, Shida S, Arima T (2006) Change of fi ne struc-ture and thermo-oxidative degradation properties of wood char-coal by heat treatment (in Japanese). Wood Carbonization Res 3:37–44
7. Iwashita T, Inagaki M (1992) Intercalation of sulfuric acid into graphite – followed by potential measurement (in Japanese). J Chem Soc Jpn 12:1412–1422
8. Maksimova NV, Sorokina NE, Shornikova ON, Avdeev VV (2004) Thermal properties of graphite intercalation compounds with acids. J Phys Chem Solid 65:177–180
9. Ishimaru K, Hata T, Bronsveld P, Nishizawa T, Imamura Y (2007) Characterization of sp2- and sp3-bonded carbon in wood charcoal.
J Wood Sci 53:442–448